# How Initial Setting Of Cement Is Found?

Final Setting Time of Cement – Final setting time of cement is the time when the paste (cement + water) completely loses its plasticity. Within final setting time, concrete hardens sufficiently to attain the predefine shape in which it is castes. After the final setting time of concrete, you can remove the form or scaffolding.

## What is initial setting time of cement?

Initial and Final Setting Time of Cement Test Procedure by Vicat Apparatus Initial and Final Setting Time of Cement Test Procedure by Vicat Apparatus Setting time of cement paste is that the interval during which the cement paste losses its plasticity after adding water in cement. Setting time of cement is calculated in two parts: (1) Initial setting time of cement and (2) Final setting time of cement.

1. Initial setting time is regarded as the time elapsed between the moments that the water is added to the cement to the time that the paste starts losing its plasticity and the hardening of the cement starts,
2. It is the time within which the cement can be molded in any desired shape without losing its strength.

The final setting time is the time elapsed between the moment when water is added to the cement and the time when the paste has completely lost its plasticity and has attained the sufficient firmness to resist certain and definite pressure. This is the time taken for the cement paste to becomes hard and attain the shape of the mould in which it is cast.

 Vicat-Apparatus-Diagram

Hi friends, you are welcomed in the world of, Read definition, apparatus, IS code, test procedure, formula, result and lab report about initial and final setting time of cement by Vicat apparatus,

1. IS: 4031 (Part 5)-1988, Methods of physical test for hydraulic cement paste
2. IS: 5513-1996, For specification for Vicat’s apparatus
1. Vicat’s apparatus conforming to IS: 5513-1976
2. Plunger
3. Glass plate
4. Weighing Balance of capacity 1000g and sensitivity to 1g.
5. Gauging trowel conforming to IS: 10086-1982.
6. Stop Watch
7. Dial Gauge

The Vicat’s apparatus for consistency test of cement paste consists of a frame having a movable rod with a cap at one end and at the other end any one of the following attachment, which are interchangeable:

• Needle for determining the initial setting time
• Needle for determining the final setting time
• Plunger for determining the standard consistency

The other two needles are made to freely fall into a Vicat mould filled with the cement paste and the amount of penetration of the needles of plunger of 10 mm diameter can be noted using the vertical graduations from 0 mm to 50 mm. Sampling and Selection of Test Specimen: The samples of the cement shall be taken as per IS: 3535- 1986* and the relevant standard specification for the type of cement being tested.

 Vicat Apparatus

Preparation of Test Block

1. Before testing the setting time of cement, do the consistency test to obtain the required quantity of water to give the paste normal consistency.
2. Prepare a neat 300 g cement paste by gauging the cement with 0.85 times the water required to give a paste of standard consistency. Potable or distilled water will be used in preparing the cement paste.
3. Take care that the time of gauging is not less than 3 minutes, not more than 5 minutes and the gauging will be completed before setting occurs.
4. The gauging time will be counted from the time of adding the water to the dry cement until starting to fill the mould. Record this time (T ₁ ).
5. Fill the Vicat mould with a cement paste gauged as above and also the mould resting on a nonporous plate.
6. Fill the mould completely and smooth off the surface of the cement paste making it level with the top of the Vicat mould.
7. In filling, the mould operators hands and the blade of the gauging trowel will only be used.
8. After moulding, immediately place the test block within the moist closet or moist room and allow it to remain there except when determinations of the time of setting are being made.

Determination of Initial Setting Time of Cement

1. Place the test block confined in the mould and resting on the non-porous plate, under the rod bearing lower the needle gently until it comes in touch with the surface of the test block and quickly release, allowing it to penetrate into the test block.
2. In. the beginning, the needle will completely pierce the test block.
3. Repeat this procedure until the needle, when brought in touch with the test block and released as described above, fails the to pierce the block beyond a point 4.5 mm to 5.5 mm measured from the bottom of the mould.
4. The period elapsing between the moments when the cement is mixed with water and the moment at which the needle fails to pierce the test block beyond a point 4.5 mm to 5.5 mm measured from the bottom of the mould will be the initial setting time of the cement paste,
5. Record this time (T ₂ ).
You might be interested:  What Is The Major Component In Building Material Cement?

Determination of Final Setting Time of Cement

1. Replace the needle of the Vicat apparatus by the needle with an annular attachment.
2. The sample of cement paste will be considered as finally set when, upon applying the needle gently to the surface of the test block, the needle makes an impression there on, while the attachment fails to do so.
3. The period elapsing between the time when the cement is mixed with water and the time at which the needle makes an impression on the surface of test block while the attachment fails to do so will be the final setting time of the cement paste,
4. Record this time (T ₃ ).

Note: In the event of a scum forming on the surface of the test block, use the underside of the block for the determination of setting time of cement.1. Type of cement =.2. Brand of cement =,3. Weight of given sample of cement is =,g 4. The normal consistency of a given sample of cement paste is =,% 5. Volume of the water added for preparation of test block = ml

Initial setting time = T ₂ – T ₁ Final setting time = T ₃ – T ₁ T ₁ = Time at which water is first added to cement T ₂ = Time when needle fails to penetrate 5 mm to 7 mm from bottom of the mould T ₃ = Time when the needle makes an impression but the attachment fails to do so.1.

1. Clean the apparatus thoroughly before testing and after testing.
2. The test should be performed away from vibrations and other disturbances.
3. Care should be taken to maintain the specified temperature, humidity and the time of mixing so as to avoid setting of cement paste as per test requirement.
4. Clean appliances should be used for gauging and gauging time should be strictly observed.
5. Care shall be taken to keep the needle straight and clean.
6. The initial and final setting time needles should be released gently.
7. Position of the Vicat mould should be shifted slightly after each penetration to avoid penetration at the same place.

Table: Indian Standard Specification of Cement Value of Initial and Final Setting Time for Ordinary Portland Cement (OPC): The initial setting time for OPC, SRC, PPC, RHPC and PSC is 30 minutes. The final setting time for OPC, SRC, PPC, RHPC and PSC is 600 minutes. Initial and final setting time of cement measured by:- Initial and final setting time of cement measured by vicat’s apparatus.

#### What is final setting time of cement paste?

Initial and Final Setting Time of Cement Test Procedure by Vicat Apparatus Initial and Final Setting Time of Cement Test Procedure by Vicat Apparatus Setting time of cement paste is that the interval during which the cement paste losses its plasticity after adding water in cement. Setting time of cement is calculated in two parts: (1) Initial setting time of cement and (2) Final setting time of cement.

• Initial setting time is regarded as the time elapsed between the moments that the water is added to the cement to the time that the paste starts losing its plasticity and the hardening of the cement starts,
• It is the time within which the cement can be molded in any desired shape without losing its strength.

The final setting time is the time elapsed between the moment when water is added to the cement and the time when the paste has completely lost its plasticity and has attained the sufficient firmness to resist certain and definite pressure. This is the time taken for the cement paste to becomes hard and attain the shape of the mould in which it is cast.

You might be interested:  How To Calculate Cement In Brick Masonry?
 Vicat-Apparatus-Diagram

Hi friends, you are welcomed in the world of, Read definition, apparatus, IS code, test procedure, formula, result and lab report about initial and final setting time of cement by Vicat apparatus,

1. IS: 4031 (Part 5)-1988, Methods of physical test for hydraulic cement paste
2. IS: 5513-1996, For specification for Vicat’s apparatus
1. Vicat’s apparatus conforming to IS: 5513-1976
2. Plunger
3. Glass plate
4. Weighing Balance of capacity 1000g and sensitivity to 1g.
5. Gauging trowel conforming to IS: 10086-1982.
6. Stop Watch
7. Dial Gauge

The Vicat’s apparatus for consistency test of cement paste consists of a frame having a movable rod with a cap at one end and at the other end any one of the following attachment, which are interchangeable:

• Needle for determining the initial setting time
• Needle for determining the final setting time
• Plunger for determining the standard consistency

The other two needles are made to freely fall into a Vicat mould filled with the cement paste and the amount of penetration of the needles of plunger of 10 mm diameter can be noted using the vertical graduations from 0 mm to 50 mm. Sampling and Selection of Test Specimen: The samples of the cement shall be taken as per IS: 3535- 1986* and the relevant standard specification for the type of cement being tested.

 Vicat Apparatus

Preparation of Test Block

1. Before testing the setting time of cement, do the consistency test to obtain the required quantity of water to give the paste normal consistency.
2. Prepare a neat 300 g cement paste by gauging the cement with 0.85 times the water required to give a paste of standard consistency. Potable or distilled water will be used in preparing the cement paste.
3. Take care that the time of gauging is not less than 3 minutes, not more than 5 minutes and the gauging will be completed before setting occurs.
4. The gauging time will be counted from the time of adding the water to the dry cement until starting to fill the mould. Record this time (T ₁ ).
5. Fill the Vicat mould with a cement paste gauged as above and also the mould resting on a nonporous plate.
6. Fill the mould completely and smooth off the surface of the cement paste making it level with the top of the Vicat mould.
7. In filling, the mould operators hands and the blade of the gauging trowel will only be used.
8. After moulding, immediately place the test block within the moist closet or moist room and allow it to remain there except when determinations of the time of setting are being made.

Determination of Initial Setting Time of Cement

1. Place the test block confined in the mould and resting on the non-porous plate, under the rod bearing lower the needle gently until it comes in touch with the surface of the test block and quickly release, allowing it to penetrate into the test block.
2. In. the beginning, the needle will completely pierce the test block.
3. Repeat this procedure until the needle, when brought in touch with the test block and released as described above, fails the to pierce the block beyond a point 4.5 mm to 5.5 mm measured from the bottom of the mould.
4. The period elapsing between the moments when the cement is mixed with water and the moment at which the needle fails to pierce the test block beyond a point 4.5 mm to 5.5 mm measured from the bottom of the mould will be the initial setting time of the cement paste,
5. Record this time (T ₂ ).

Determination of Final Setting Time of Cement

1. Replace the needle of the Vicat apparatus by the needle with an annular attachment.
2. The sample of cement paste will be considered as finally set when, upon applying the needle gently to the surface of the test block, the needle makes an impression there on, while the attachment fails to do so.
3. The period elapsing between the time when the cement is mixed with water and the time at which the needle makes an impression on the surface of test block while the attachment fails to do so will be the final setting time of the cement paste,
4. Record this time (T ₃ ).
You might be interested:  Dental Filling Is Done By Which Cement?

Note: In the event of a scum forming on the surface of the test block, use the underside of the block for the determination of setting time of cement.1. Type of cement =.2. Brand of cement =,3. Weight of given sample of cement is =,g 4. The normal consistency of a given sample of cement paste is =,% 5. Volume of the water added for preparation of test block = ml

Initial setting time = T ₂ – T ₁ Final setting time = T ₃ – T ₁ T ₁ = Time at which water is first added to cement T ₂ = Time when needle fails to penetrate 5 mm to 7 mm from bottom of the mould T ₃ = Time when the needle makes an impression but the attachment fails to do so.1.

1. Clean the apparatus thoroughly before testing and after testing.
2. The test should be performed away from vibrations and other disturbances.
3. Care should be taken to maintain the specified temperature, humidity and the time of mixing so as to avoid setting of cement paste as per test requirement.
4. Clean appliances should be used for gauging and gauging time should be strictly observed.
5. Care shall be taken to keep the needle straight and clean.
6. The initial and final setting time needles should be released gently.
7. Position of the Vicat mould should be shifted slightly after each penetration to avoid penetration at the same place.

Table: Indian Standard Specification of Cement Value of Initial and Final Setting Time for Ordinary Portland Cement (OPC): The initial setting time for OPC, SRC, PPC, RHPC and PSC is 30 minutes. The final setting time for OPC, SRC, PPC, RHPC and PSC is 600 minutes. Initial and final setting time of cement measured by:- Initial and final setting time of cement measured by vicat’s apparatus.

## Why does cement take a long time to set in sand?

The fineness of cement, the presence of salts in sand, atmospheric conditions. For example, cement requires a temperature of 27°c to complete Hydration, during winters the climate is low which stops the hydration and takes a longer time to set harden. As Per IS: 4031 (Part 5) – 1988.

#### When is the cement assmed as finally set?

Procedure:- –

Take 400g of cement and place it in a bowl or tray.Now add water of Start the stopwatch at the moment water is added to the cement. Water of quantity 0.85P.times (Where P is the Standard consistency of cement ) is considered.Now fill the mix in Vicat mould. If any excessive paste remained on Vicat mould is taken off by using a trowel.Then, place the VICAT mould on non porous plate (Glass plate) and see that the plunger should touch the surface of VICAT mould gently.Release the Plunger and allow it to sink into the test mould.Note down the penetration of the plunger from the bottom of mould indicated on the scale.Repeat the same experiment at different positions on the mould until the plunger should stop penetrating 5 from the bottom of the mould.

The time period elapsed between the moment water is added to the cement and the time, the needle fails to penetrate the mould of 5mm when measured from the bottom of the mould, is the initial setting time of cement. Now replace the needle (plunger) by the one with an annular attachment. The cement is assmed as finally set When, upon applying the needle gently to the surface of the test mould, the needle makes an impression therein, while the attachment fails to do so.

• The time period between the moment water is added to the cement and the time at which needle makes an impression on the surface of the mould, while the attachment fails to do so, is the final setting time of cement.